Upload
phamlien
View
245
Download
4
Embed Size (px)
Composite Structures 131 (2015) 333–343
Contents lists available at ScienceDirect
Composite Structures
journal homepage: www.elsevier .com/locate /compstruct
XFEM buckling analysis of cracked composite plates
http://dx.doi.org/10.1016/j.compstruct.2015.05.0130263-8223/� 2015 Elsevier Ltd. All rights reserved.
⇑ Corresponding author. Tel.: +98 21 6111 2258; fax: +98 21 6640 3808.E-mail address: [email protected] (S. Mohammadi).
Amir Nasirmanesh, Soheil Mohammadi ⇑High Performance Computing Lab, School of Civil Engineering, University of Tehran, Tehran, Iran
a r t i c l e i n f o
Article history:Available online 13 May 2015
Keywords:Buckling analysisExtended finite element method (XFEM)CrackComposite plateOrthotropic tip enrichment functions
a b s t r a c t
Linear eigenvalue buckling analysis for cracked uni-layer composite plates is performed in the frameworkof the extended finite element method (XFEM). The geometry of the problem is discretized using the8-noded degenerated shell element, which includes transverse shear deformation effects. The effects ofseveral parameters such as crack lengths and angles, fiber directions and boundary conditions on thebuckling behavior of cracked composite plates are comprehensively investigated for different loadingconditions including compressive, tensile and shear loadings. Also, the accuracy and efficiency of the pro-posed method are discussed and compared with the available results.
� 2015 Elsevier Ltd. All rights reserved.
1. Introduction
Composite materials have been widely used in aerospace, mar-ine and civil engineering in the form of thin plate structures due totheir advantages such as the high ratio of strength to weight.Among several different failure modes for thin composite plates,the buckling failure can jeopardize the overall safety of the struc-ture due to sudden and large deformations that occur. In general,structural components, especially thin plates are highly suscepti-ble to buckling when they are subjected to compressive loadings.Nevertheless, the presence of flaws such as cracks in plates cancause local and even global buckling even in tensile loadings. Asa result, the presence of imperfections, such as cracks, voids andetc, during manufacturing, installation and performance not onlyreduces the stiffness and strength of plate, they highly increasethe risk of buckling even in tensile loadings by creating localmulti-axial and compressive stress states around the crack.
A number of studies are available on buckling analysis of com-posite and orthotropic plates without cracks. Thai and Kim [1] pre-sented the closed-form solution for buckling of rectangularorthotropic plates. They assumed a quadratic variation for trans-verse shear strains across the thickness. Lopatin and Morozof [2]studied the buckling of rectangular orthotropic composite platessubjected to a linearly distributed in-plane loading using thetwo-variable refined theory. They investigated the effect of aspectratio and direction of fibers on the buckling behavior and deter-mined the optimum angle of fibers. Similar studies [3–6] were per-formed on the buckling analysis of orthotropic composite plates.
Also, several studies have been performed for the analysis of com-posite plates in the framework of the isogeometric analysis, whichis capable of modeling complex geometries [7–9].
On the other hand, many researchers have studied the bucklingof cracked isotropic plates. For instance, Markström and Stoakers[10] performed a finite element analysis to study buckling ofcracked members under tension, and concluded that the criticalbuckling stress was proportional to the square of the crack length,inversely. A similar study was performed in [11] using singular tipelements. Riks et al. [12] demonstrated that the stress intensityfactors increased around the crack tips dramatically when bucklingoccurred. The integral equation method was applied by Vafai et al.[13] to study the edge cracked plates under in-plane compressiveperiodic loading. Experimental and numerical buckling analysisof isotropic cracked rectangular plates under compressive and ten-sile loading were performed by Seifi and Kabiri [14] and Seifi andKhoda-yari [15], while shear buckling and post-buckling analysisof cracked panels were studied by Alinia et al. [16] using the finiteelement method. They showed that the accuracy of the resultswere highly sensitive to mesh density at crack tips. Other workson isotropic plates can be found in [17–20]. Natarajan et al. [21]developed an XFEM model to solve the buckling problem of isotro-pic cracked plates using a plate element with smooth curvatures.Free vibration analysis of cracked functionally graded plates wasperformed by Natarajan et al. based on XFEM and using a4-noded quadrilateral plate element [22]. They investigated theeffect of crack length, crack location, crack orientation, gradientindex of material and the thickness of plate on the natural frequen-cies and mode shapes of the plate. Recently, Nguyen-Thoi et al. [23]studied the problem of free vibration analysis of cracked Mindlinplates using the extended cell-based smoothed discrete shear gap
Fig. 1. Geometry of the 8 noded shell element.
334 A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343
method (XCS-DSG3). They concluded that the proposed methodhad a high accuracy in comparison to other conventional plate ele-ments. Another study about extended discrete shear gap methodcan be found in [24].
There is, however, only a very limited literature on the bucklinganalysis of cracked orthotropic plates. Barut et al. [25] presented anumerical study on buckling and post-buckling of laminated com-posite plates with an inclined crack subjected to tension using a geo-metrical nonlinear finite element method. The effect of layersequence on the critical buckling stress was also studied. In theirproposed method, elements should conform to crack faces, prevent-ing simulation of arbitrary crack propagations. Recently, Rad andPanahandeh-Shahraki [26] studied the buckling of functionallygraded plates subjected to uni-axial and bi-axial tensile loads bymeans of the finite element method. They concluded that the buck-ling load decreased by the increase of gradient index of material andthis attitude was more sensitive for bi-axial loadings. Similarly, aparametric study was performed, using partition of unity method,to investigate the effect of discontinuities in the functionally gradedmaterial plates [27], showing that with increasing material gradientindex and crack length, the buckling load would decrease. It shouldbe noted that they used isotropic tip enrichment functions for tipelements. None of the existing works has studied the problem ofbuckling of cracked orthotropic plates subjected to general loadingconditions with the extended finite element method. In this study,XFEM is adopted for buckling analysis of several mixed-modecracked composite plates for the first time. The orthotropic cracktip enrichment functions [28] are considered to model the stress sin-gularity in a more accurate manner.
XFEM has been developed in the past decade to alleviate theshortcomings of the finite element method in discontinuous prob-lems, by avoiding the need of conforming the discontinuity to themesh edges and also adopting singular elements for reproducingthe stress singularity at crack tips. This method has successfullybeen extended to several static and dynamic isotropic and ortho-tropic problems, as well as modeling inter laminar cracks inbi-materials [22,28–38]. Recently, Nguyen-Thanh et al. [39] devel-oped an extended isogeometric shell formulation based on theKirchhoff–Love theory. More advanced methods related to theproblem of cracked shells can be found in [40,41]. Also, For a com-prehensive review of XFEM developments, see [42,43].
The structure of the paper is as follows: the fundamental equa-tions of the shell element and the buckling eigenvalue equationsare discussed in the framework of XFEM formulation with anemphasize on isotropic and orthotropic crack tip enrichment func-tions. Several numerical examples are presented and discussed inSection 3, beginning with verifications and then extension to ortho-tropic composite plates. The last part of the paper presents theresults for the buckling analysis of various cracked composite plates.
2. Basic formulation
In the present study, eight noded shell elements based on theMindlin–Reissner theory are used to discretize the model. Theseelements have many advantages such as avoiding mesh distortionand shear locking in thin plates and shells. The geometry of theshell element is interpolated using
xy
z
8><>:
9>=>; ¼
Xn
i¼1
Niðn;gÞxi
yi
zi
8><>:
9>=>;þ
t2
Xn
i¼1
fNiðn;gÞV3
xi
V3yi
V3zi
8>><>>:
9>>=>>; ð1Þ
where t is the thickness of the shell element, Niðn;gÞ are the conven-tional shape functions in the natural coordinate system, n ¼ 8 is thenumber of nodes in the element, V3
i is the unit normal vector at
node i and f is perpendicular to the mid-surface in the natural coor-dinate system (Fig. 1).
Taking into account the shear deformation effects, approxima-tion of the displacement field can be expressed in terms of nodaldisplacements and rotations,
ufem ¼Xn
i¼1
Niui �t2
Xn
i¼1
Nifexiai þt2
Xn
i¼1
Nifeyibi ð2Þ
where exi and eyi are the orthonormal vectors of unit normal vectorat node i, as depicted in Fig. 1, ai and bi are rotations with respect tox and y directions, respectively, and
uT ¼ u;v ;wf g ð3Þ
u; v and w are the displacement components in x; y and z direc-tions, respectively. The standard vector of unknowns d
�is defined as,
d�¼ u; v;w;a;bf gT ð4Þ
Now, let us consider a crack in an orthotropic uni-layer compos-ite plate, as shown in Fig. 2. The general form of XFEM approxima-tion for the displacement field of any point x is defined as:
u�¼ ufem þ uenrich ð5Þ
On the right hand side of this equation, the first part is the con-ventional finite element approximation and the second part isadded in order to consider the crack face discontinuity and thestress singularity at crack tips
uenrich ¼ ucrack-face þ ucrack-tip ð6Þ
where ucrack-face enriches the displacement field with the Heavisidefunction so that the discontinuity along the crack edges is modeled
ucrack-face ¼Xn
i¼1
NiHðxÞai þt2
Xn
i¼1
fNiHðxÞ �exiaai þ eyiabi� �
ð7Þ
where
ai ¼ aui ; a
vi ; a
wi
� �T ð8Þ
It should be noted that ai; aai and abi are the additional enrich-ment degrees of freedom. The enrichment vector of degrees of free-dom h can be written as,
h ¼ aui ; a
vi ; a
wi ; aai; abi
� �T ð9Þ
The Heaviside function for a point x is defined as [42]
HðxÞ ¼þ1 x above the crack�1 x under the crack
�ð10Þ
The term ucrack-tip in Eq. (5) is added to enrich the displacementfield to capture the stress singularity at the crack tip,
ucrack-tip ¼Xnt
i¼1
Ni
Xm
j¼1
ðFjðxÞ�FjðxiÞÞbu
i
bvi
0
8><>:
9>=>;þ
Xnt
i¼1
Ni
Xm
j¼1
ðGjðxÞ�GjðxiÞÞ00bw
i
8><>:
9>=>;
þXnt
i¼1
Nifti
2
Xm
j¼1
ðRjðxÞ�RjðxiÞÞ �exibjaiþeyib
jbi
h ið11Þ
Fig. 2. A cracked orthotropic medium.
A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343 335
where m is the number of tip enrichment functions and nt is the
number of nodes enriched by the crack tip functions, while b ji ; b
jai
and b jbi are additional degrees of freedom, presented as
t ¼ bui ; b
vi ; b
wi ; bai; bbi
� �T ð12Þ
In Eq. (11), F;G and R are the in-plane, out of plane and rota-tional tip enrichment functions, respectively [32]. Isotropic andorthotropic in-plane tip enrichment functions are considered forisotropic and composite problems, respectively.
According to [28], the following in-plane orthotropic tip enrich-ment functions are considered
F r; hð Þ ¼ffiffiffirp
cos h12
� ffiffiffiffiffiffiffiffiffiffiffig1 hð Þ
p;ffiffiffirp
cos h22
� ffiffiffiffiffiffiffiffiffiffiffig2 hð Þ
p;ffiffiffi
rp
sin h12
� ffiffiffiffiffiffiffiffiffiffiffig1 hð Þ
p;ffiffiffirp
sin h22
� ffiffiffiffiffiffiffiffiffiffiffig2 hð Þ
p( )
ð13Þ
gj hð Þ ¼ cos hð Þ þ cj sinðhÞ �2
þ bj sinðhÞ� 2
� 1=2
; j ¼ 1;2 ð14Þ
hk hð Þ ¼ arctanbksinðhÞ
cos hð Þ þ cksinðhÞ
� ; k ¼ 1;2 ð15Þ
where cj and bj are obtained from the roots of the following charac-teristic equation [44]
ptip11l
4 � 2ptip16l
3 þ 2ptip12 þ ptip
66
�l2 � 2ptip
26lþ ptip22 ¼ 0 ð16Þ
l1 ¼ c1 þ ib1
l2 ¼ c2 þ ib2ð17Þ
and pij are the components of the compliance tensor p which iscomputed from the tensor of material properties C,
C ¼
C11 C12 C13 0 0 0C21 C22 C23 0 0 0C31 C32 C33 0 0 00 0 0 C44 0 00 0 0 0 C55 00 0 0 0 0 C66
2666666664
3777777775
ð18Þ
p ¼ C�1 ð19Þ
In the case of isotropic problems, the classical in-plane isotropictip enrichment functions are employed [42]
F r;hð Þ¼ffiffiffirp
sinh2
� ;ffiffiffirp
cosh2
� ;ffiffiffirp
sinh2
� sin hð Þ;
ffiffiffirp
cosh2
� sin hð Þ
� �ð20Þ
Out of plane and rotational enrichment functions are [32]
Gðr; hÞ ¼ffiffiffirp
sinh2
� ; r3=2 sin
h2
� ; r3=2 cos
h2
� ;
�
r3=2 sin3h2
� ; r3=2 cos
3h2
� �ð21Þ
R r; hð Þ ¼ffiffiffirp
sinh2
� ;ffiffiffirp
cosh2
� ;ffiffiffirp
sinh2
� sin hð Þ;
�
r cosh2
� sin hð Þ
r �ð22Þ
According to [32], without the loss of accuracy, the out planeenrichment functions can be further simplified to
Gðr; hÞ ¼ffiffiffirp
sinh2
� � �ð23Þ
The total potential energy P is used to derive the final form ofthe governing equation,
P ¼ 12
ZveT
L CeLdV þZ
veT
NLr0dV ð24Þ
where C is the tensor of material properties, eL and eNL are the linearand nonlinear parts of Green–Lagrange strain,
e ¼ eL þ eNL ¼ ex; ey; ez; cxy; cxz; cyz
n oTð25Þ
eL ¼12
@u� i
@xjþ@u� j
@xi
!ð26Þ
eNL ¼12
@u�k
@xi
@u�k
@xj; i; j; k ¼ 1;2;3 ð27Þ
where the indices 1, 2 and 3 are related to x, y and z directions,respectively. r0 is the stress state computed from the linear staticanalysis,
r0 ¼ rx0;ry0;rz0; sxy0; syz0; sxz0� �T ð28Þ
r0 is then used to evaluate the geometric stiffness matrix, associ-ated with the second part of P.
Satisfying the principle of minimum potential energy requiresthe variation of P to vanish (dP ¼ 0 ). After some manipulation,the stability equation is obtained as
Kþ kKGð Þ Df g ¼ 0 ð29Þ
Eq. (29) is an eigenvalue equation, where k represents theeigenvalue and D is the corresponding eigenvector; the bucklingmode shapes,
D ¼ d�
h t1 t2 t3 t4
n oT
The smallest value of k determines the critical buckling stress. Kand KG are the standard and geometric stiffness matrices,respectively,
Krsij ¼
ZvðBr
i ÞT CBs
j dV ð30Þ
KrsG ij ¼
ZvðBr
G iÞT S0ðBs
G jÞdV ðr; s ¼ d;h; tÞ ð31Þ
and S0 is the matrix of stress components of r0 , computed from thestatic analysis
336 A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343
S0 ¼S0 0 00 S0 00 0 S0
264
375 ð32Þ
S0 ¼rx0 sxy0 sxz0
sxy0 ry0 syz0
sxz0 syz0 rz0
264
375 ð33Þ
Bd can be obtained from [45]
Bdi ¼
@Ni@x 0 0 @
@x �ft2 ex1Ni
� @@x
ft2 ey1Ni�
0 @Ni@y 0 @
@y �ft2 ex2Ni
� @@y
ft2 ey2Ni�
0 0 @Ni@z
@@z �
ft2 ex3Ni
� @@z
ft2 ey3Ni�
@Ni@y
@Ni@x 0
@@y �
ft2 ex1Ni
� þ @
@yft2 ey1Ni�
þ@@x �
ft2 ex2Ni
� @@x
ft2 ey2Ni�
0 @Ni@z
@Ni@y
@@z �
ft2 ex2Ni
� þ @
@zft2 ey2Ni�
þ@@y �
ft2 ex3Ni
� @@y
ft2 ey3Ni�
@Ni@z 0 @Ni
@x
@@z �
ft2 ex1Ni
� þ @
@zft2 ey1Ni�
þ@@x �
ft2 ex3Ni
� @@x
ft2 ey3Ni�
266666666666666666664
377777777777777777775
ð34Þ
To obtain the components of Bhi ;Ni should be replaced with
Ni HðxÞ � HðxiÞð Þ in Eq. (34).Bt is composed of four components,
Bti ¼ Bt1
i Bt2i Bt3
i Bt4i
� �ð35Þ
and each component Btji , which is related to one of the specific tip
enrichment functions, is computed as
Bti ¼
@/@x 0 0 @
@x �ft2 ex1u
� @@x
ft2 ey1u�
0 @/@y 0 @
@y �ft2 ex2u
� @@y
ft2 ey2u�
0 0 @j@z
@@z �
ft2 ex3u
� @@z
ft2 ey3u�
@/@y
@/@x 0
@@y �
ft2 ex1u
� þ @
@yft2 ey1u�
þ@@x �
ft2 ex2u
� @@x
ft2 ey2u�
0 @/@z
@j@y
@@z �
ft2 ex2u
� þ @
@zft2 ey2u�
þ@@y �
ft2 ex3u
� @@y
ft2 ey3u�
@/@z 0 @j
@x
@@z �
ft2 ex1u
� þ @
@zft2 ey1u�
þ@@x �
ft2 ex3u
� @@x
ft2 ey3u�
266666666666666666664
377777777777777777775
ð36Þ
where /;u and j are
/ ¼ Ni Fj xð Þ � Fj xið Þ�
ð37Þ
u ¼ Ni Rj xð Þ � Rj xið Þ�
ð38Þ
j ¼ Ni Gj xð Þ � Gj xið Þ�
ð39Þ
The geometric matrix BdGi can be written as [45],
BdGi ¼
@Ni@x 0 0 @
@x �ft2 ex1Ni
� @@x
ft2 ey1Ni�
@Ni@y 0 0 @
@y �ft2 ex1Ni
� @@y
ft2 ey1Ni�
@Ni@z 0 0 @
@z �ft2 ex1Ni
� @@z
ft2 ey1Ni�
0 @Ni@x 0 @
@x �ft2 ex2Ni
� @@x
ft2 ey2Ni�
0 @Ni@y 0 @
@y �ft2 ex2Ni
� @@y
ft2 ey2Ni�
0 @Ni@z 0 @
@z �ft2 ex2Ni
� @@z
ft2 ey2Ni�
0 0 @Ni@x
@@x �
ft2 ex3Ni
� @@x
ft2 ey3Ni�
0 0 @Ni@y
@@y �
ft2 ex3Ni
� @@y
ft2 ey3Ni�
0 0 @Ni@z
@@z �
ft2 ex3Ni
� @@z
ft2 ey3Ni�
2666666666666666666664
3777777777777777777775
ð40Þ
BhGi is determined by replacing Ni with Ni HðxÞ � HðxiÞð Þ in Eq. (40),
and BtGi is obtained as
BtGi ¼
@/@x 0 0 @
@x �ft2 ex1u
� @@x
ft2 ey1u�
@/@y 0 0 @
@y �ft2 ex1u
� @@y
ft2 ey1u�
@/@z 0 0 @
@z �ft2 ex1u
� @@z
ft2 ey1u�
0 @/@x 0 @
@x �ft2 ex2u
� @@x
ft2 ey2u�
0 @/@y 0 @
@y �ft2 ex2u
� @@y
ft2 ey2u�
0 @/@z 0 @
@z �ft2 ex2u
� @@z
ft2 ey2u�
0 0 @j@x
@@x �
ft2 ex3u
� @@x
ft2 ey3u�
0 0 @j@y
@@y �
ft2 ex3u
� @@y
ft2 ey3u�
0 0 @j@z
@@z �
ft2 ex3u
� @@z
ft2 ey3u�
266666666666666666664
377777777777777777775
ð41Þ
Evaluation of standard and geometric stiffness matrices, K andKG, requires accurate integration of Eqs. (30) and (31). Amongseveral methods for numerical evaluation of these integrals[16,46–50], the sub-triangulation technique along with the Gaussquadrature rule is adopted in this study [43]. For elements enrichedwith the Heaviside function, 7 Gauss points are used in each trian-gle. In the tip elements, due to the presence of stress singularity inthe vicinity of crack tip, 13 Gauss points are employed per triangle.For other elements, an ordinary 2� 2 Gaussian quadrature rule isconsidered. The two different type of tip and split elements and theircorresponding enriched nodes are shown in Fig. 3.
3. Numerical examples
In this section, linear eigenvalue buckling analyses are per-formed for five different problems in two cases of isotropic andorthotropic uni-layer composite plates. The effects of differentparameters such as the aspect ratio, boundary conditions, cracklength, crack angle and orthotropic angle on the buckling loadand mode shapes are investigated. The problems include a crackedrectangular plate under uniform compressive, tensile and shearloading conditions, circular cracked plate with two concentratedtensile point loads and a square plate with two parallel cracksunder tensile loading. Due to the fact that there is no documentedinformation on the buckling of cracked fiber composite plates, themethod is first verified for the isotropic cases available in the liter-ature and then comprehensively examined for orthotropicproblems.
For discretizing the model, eight-noded degenerated shell ele-ments are considered and the reduced integration technique isadopted to avoid potential shear locking. Two sets of in-plane tipenrichment functions, Eqs. (13) and (20), are used for the orthotro-pic and isotropic problems, respectively.
The adopted mechanical properties for all orthotropic compos-ite problems considered in this study are presented in Table 1. In
Fig. 3. Different element types and enriched nodes.
Table 1Mechanical properties of composite material.
E1ðMPaÞ E2ðMPaÞ E3ðMPaÞ G12ðMPaÞ G13ðMPaÞ G23ðMPaÞ m12 m13 m23
206842 20684.2 20684.2 6894.7 6894.7 4136.8 0.3 0.25 0.25
Fig. 4. Geometry and mesh of the plate.
Table 2Critical buckling loads for the isotropic plate subjected to compressive loading.
c a BC h� Mode I buckling load (N) Error %
EXP. [12] FEM. [12] XFEM FEM XFEM
1 0.1 CC 0 1627 1765.8 1682.3 8.5 3.41 0.3 CC 0 1531 1602.5 1560.8 4.7 21 0.3 CC 30 1551 1669.7 1630.1 7.7 5.11 0.5 CC 60 1636 1701.3 1694.9 4 3.61 0.5 CC 90 1665 1765.8 1738.3 6.1 4.41.33 0.3 CC 0 1158 1217.7 1191.6 5.2 2.92 0.5 CC 30 725 792.7 754 9.3 41 0.3 SC 0 815 835.7 833.8 2.5 2.31 0.3 SS 0 404 384.9 406.3 �4.7 0.61 0.5 SS 30 387 359.2 390.5 �7.2 0.9
Fig. 5. Effect of the crack angle on the buckling stress.
Fig. 6. The first four buckling mode shapes for the horizontally (a) and vertically (b)cracked composite plates.
A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343 337
the case of isotropic problems, the mechanical properties aredefined separately for each problem.
3.1. Cracked rectangular plate under compression
3.1.1. Isotropic plateA cracked rectangular plate subjected to a uniform in-plane
compressive load was tested experimentally by Seifi andKhoda-yari [15] and then numerically simulated by the classicalfinite element method. The geometry of plate and loading condi-tion as well as the typical structured finite element mesh (1225elements) are shown in Fig. 4. Thickness of the plate is
t ¼ 1:2 mm;E ¼ 70 GPa and m ¼ 0:3. The extended finite elementmethod with isotropic crack tip enrichment functions is adoptedto perform the numerical simulations.
Four different boundary conditions are considered for plateedges. In all cases, the right and left edges of rectangular platesare free, whereas the other edges are either clamped (C) or simplysupported (S), as depicted in Fig. 4.
Fig. 7. Effect of orthotropic angle on the buckling stresses.
338 A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343
Table 2 compares the predicted critical stresses associated withthe first mode of buckling for different cases of crack lengths andangles, aspect ratios and boundary conditions.
Clearly, the buckling loads predicted by XFEM are in betteragreement with the experimental results. All simulations havebeen performed on a fixed mesh of 1225 elements and 3816 nodes,showing the efficiency of the present extended finite element mod-eling in comparison with the classical finite element method. Itshould be noted that Ref. [15] used 2157 elements and 6603 nodesto model the case of c ¼ 1 , a ¼ 0:3; h ¼ 0� and CC boundary condi-tions; almost two times the number of DOFs of present XFEM.
3.1.2. Orthotropic composite plateIn this section, buckling stresses for cracked orthotropic plates
subjected to uniform compression are computed using a lineareigenvalue buckling analysis. Similarly, the effects of crack lengthand angle, direction of fibers and the aspect ratio of plate on thebuckling stresses and mode shapes are studied and discussed indetail. It should be mentioned that the in-plane orthotropic enrich-ment functions are applied for modeling the stress singularity atthe crack tip.
Effect of crack angleFirst, the major orthotropic direction is assumed in the x direc-
tion and then the crack angle is changed. The plate dimensions areW ¼ L ¼ 240 mm, the thickness is t ¼ 1 mm and the boundarycondition is SC.
According to Fig. 5, increasing the crack length leads to reduc-tion of buckling stress, e.g. the buckling stress for a=W ¼ 0:3 is1.58 times greater than the case of a=W ¼ 0:8. In addition, increas-ing the angle of crack increases the buckling stress up to h ¼ 60�
and then decreases.To investigate the effect of crack angle on the buckling mode
shapes, the first four mode shapes corresponding to h ¼ 0� andh ¼ 90� cracks (a ¼ 0:7Þ and their associated buckling stresses areshown in Fig. 6. Clearly, the crack angle affects the buckling behav-ior of the plate so that in higher modes, the plate buckles in a dra-matically different pattern.
Table 3Critical buckling stresses for different crack lengths, aspect ratios and several fiberangles.
a c b
0� 15� 30� 45� 60� 90�
Mode I buckling stress (Mpa)
0.3 1 1.65 1.54 1.33 1.46 2.98 6.630.3 1.33 1.63 1.51 1.26 1.34 2.82 6.390.3 2 1.61 1.49 1.17 1.19 2.7 6.340.8 1 1.03 0.97 0.82 0.81 1.51 3.210.8 1.33 1.12 1.05 0.88 0.89 1.67 3.220.8 2 1.22 1.13 0.91 0.92 1.91 4
Effect of orthotropic angle and the aspect ratio of plateIn this case, the crack angle is kept constant (h ¼ 0�Þ, but the
fibers orientation varies between 0� 6 b 6 90�. According toFig. 7 the following conclusions can be made: for low fiber orienta-tions, the buckling stresses are decreased with increasing the angleof fibers so that the most critical case is achieved at b ¼ 45�.Afterward, this attitude is reversed and with increasing the direc-tion of fibers the buckling stresses are increased. Moreover, thebuckling behavior is more sensitive to the orientation of the fibersafter b ¼ 45�.
Table 3 compares the results of buckling stresses for two differ-ent horizontal crack lengths.
Expectedly, for small crack lengths (a ¼ 0:3Þ, the buckling stressdecreases when the aspect ratio is increased, whereas for longcrack lengths (a ¼ 0:8Þ increasing the aspect ratio leads to theincrease of the buckling stress.
In order to study the mesh sensitivity of results, several mesheswith different number of elements are considered for the case ofb ¼ 90�; h ¼ 0� and a ¼ 0:8. The predicted buckling stresses, shownin Fig. 8, clearly indicate that by increasing the number of ele-ments, a converged solution of 3:15 Mpa is obtained for the buck-ling stress.
3.2. Cracked rectangular plate under tension
A cracked rectangular plate subjected to tension can locallybuckle around the crack faces due to existing local compressivestresses [12]. Seifi and Kabiri [14] evaluated the loads of isotropicplates experimentally and numerically by the classical finite ele-ment method. The geometry of the plate is shown in Fig. 4, andthe analysis is performed for both isotropic and composite casesby a structured mesh of 1225 elements.
3.2.1. Isotropic plateThe mechanical material properties are similar to isotropic case
of problem 3.1.1. The boundary conditions on the top and bottomedges are free and clamped (FC), respectively [14] and the thick-ness of the plate is t ¼ 1 mm.
The critical buckling loads for different aspect ratios, cracklengths and angles are determined and presented in Table 4.Clearly, XFEM predicts more accurate results than the classicalFEM. In addition, the present approach is more efficient becauseof using substantially less elements with a constant size of6.8 mm, while, the reference was based on an extremely finermesh with the maximum size of 3 mm and the minimum size ofapproximately 0.3 mm around the crack tip.
3.2.2. Orthotropic composite plateNow, the same problem is solved for the orthotropic composite
plate. The dimensions of the plate are W ¼ L ¼ 240 mm and
Fig. 8. Variation of the buckling stress for different mesh refinement.
Table 4Critical buckling loads for the tensile isotropic plate for different values of aspectratio, crack length and crack angle.
c a h Buckling load (N) Differencewith EXP (%)
EXP. [11] FEM. [11] XFEM FEM XFEM
1 0.5 0 6361 6820.3 6694.6 6.7 2.11 0.6 15 4614.7 5204.6 4748.5 11.3 2.91 0.7 30 5592 5765.3 5697.2 3 1.91.3 0.5 0 8208.4 7998.7 8495.7 �2.6 3.51.3 0.6 15 6207.9 5897.3 6350.7 �5.3 2.31.3 0.7 30 5700.3 6220.8 5797.3 8.4 1.7
A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343 339
t ¼ 1 mm. The mechanical properties are identical to Table 1. Theeffects of various parameters such as the crack length and angle,direction of fibers and different boundary conditions on the buck-ling stresses and mode shapes are investigated. Three types ofboundary conditions are considered:
Type A: top and bottom edges are clamped, left and right edgesare free.Type B: top and bottom edges are clamped, left and right edgesare restrained just for out of plane displacement and free forin-plane displacements.Type C: similar to Type B except that the displacements in the xdirection are restrained for the left and right edges.
Effect of crack length and orthotropic angleVarious crack lengths and orthotropic angles are considered in
this section and their effects on the buckling stress are investi-gated, as shown in Fig. 9. Type A boundary condition is consideredfor the analyses.
It is observed that with increasing the crack length, the criticalbuckling stress is substantially decreased. Also, the buckling stressfirst varies in a decreasing trend up to b ¼ 45� and then follows anincreasing path with further increase of the angle of fibers.
The buckling mode shapes related to fiber orientations of b ¼ 0�
and b ¼ 30� are presented in Fig. 10, which clearly shows that theangle of fibers can significantly change the buckling behavior ofplate in different modes.
Effect of boundary condition and crack angleTable 5 compares the buckling stresses for three different
boundary conditions in terms of different crack angles. The resultsare obtained for a ¼ 0:8; t ¼ 1 mm and b ¼ 0�. According to theresults, no significance difference is observed between Type Aand B because in these cases the local buckling of crack edgesdepends highly on the compressive in-plane stress distributionaround the crack faces and the restraint condition of out of planemovements at edges of the plate does not largely affect the
Fig. 9. Effect of fiber directions on the buckling stresses.
in-plane stress distribution under this loading condition. On theother hand, the effect of in-plane displacements at edges of theplate (Type C) can crucially affect the stress distribution aroundthe crack faces and therefore, buckling stresses become totally dif-ferent from the other types (Fig. 11).
In addition, the critical buckling stresses are dramaticallyincreased by increasing the crack angle, as depicted in Fig. 11.Finally, it is noted that at h ¼ 90� no compressive stress is gener-ated in the present tensile configuration and the plate does notbuckle, globally or locally.
From the presented results, it can be inferred that cracked com-posite plates are highly susceptible to buckling. Among the studiedproblems, the most vulnerable case is associated with the 45�
inclined fibers. Therefore, necessary measures need to be consid-ered for practical engineering designs. On the other hand, presenceof appropriate supports at plate edges can significantly improve itsbuckling behavior.
3.3. Edge cracked shear panel
The buckling analysis of a cracked shear panel, previously stud-ied by Alinia et al. [16], is considered, as shown in Fig. 12. Theyused denser adaptive mesh around the crack tip with the minimumsize of approximately 0:5 mm and the maximum size of 25 mm forother regions, whereas here a uniform extended finite elementmesh with the size of 28:6 mm is used for modeling the edgecracked shear panel. First, the isotropic case is studied and the lin-ear eigenvalue buckling analysis is performed and the obtainedresults are compared with the reference results. Then, the ortho-tropic composite case is considered and the effects of differentorthotropic angles and crack lengths on the buckling behavior ofthe plate are examined.
3.3.1. Isotropic plateSimilar to previous problems, a structured mesh with 1225 ele-
ments and 3816 nodes is adopted to discretize the model and tocompute the buckling shear stress. Material properties, boundary
Fig. 10. The first three buckling mode shapes for (a)b ¼ 0� and (b)b ¼ 30� .
Table 5Buckling stresses for various crack angles and boundary conditions.
h� Buckling stress (Mpa)
Type A Type B Type C
0 8.3 10.0 61.215 8.5 9.1 96.230 14.0 14.3 130.445 20.6 21.3 159.6
340 A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343
condition and the dimensions of the plate are identical with [16],W ¼ L ¼ 1000 mm; t ¼ 3 mm;E ¼ 210 GPa and t ¼ 0:3.
Comparison of the predicted results with the reference data, asillustrated in Fig. 13, shows a very good agreement. The referenceresults [16] used substantially more elements than the presentmethod, showing the efficiency of the present XFEM.
3.3.2. Orthotropic plateThe same plate of Fig. 12 with dimensions of L ¼W ¼ 1000 mm
and t ¼ 3 mm is considered. The material properties are accordingto Table 1. Linear eigenvalue buckling analysis is performed for theedge cracked panel and the effects of fiber orientation and cracklength on the buckling shear stresses and mode shapes areinvestigated.
Variations of the buckling shear stress with respect to fiberdirections are shown in Fig. 14, which shows a decreasing trendwith the increasing angle up to b ¼ 45�. As a result, the bucklingshear stress for the case of a=W ¼ 0:4 and b ¼ 0� is about 3 timesgreater than the case of a=W ¼ 0:7. Moreover, the most criticalfiber direction is related to b ¼ 45�, and when the fibers are parallelto the crack (b ¼ 90�Þ, the buckling behavior is improved and thebiggest buckling stress is achieved.
In order to show the effect of fiber directions on the bucklingmode shapes, the first three buckling mode shapes for the case ofa=W ¼ 0:7 and angles of fibers b ¼ 0� and b ¼ 90� are presentedin Fig. 15.
3.4. Buckling analysis of cracked composite circular plate
The other example is dedicated to a simply supported crackedcomposite circular plate subjected to two concentrated point loads.Earlier, this problem was considered by Asadpoure andMohammadi [28] to calculate the static stress intensity factorsfor different crack orientations. Now, the buckling analysis of thisproblem is performed in the framework of extended finite elementmethod. The material properties are similar to Table 1 and the ratioof the radius to the plate thickness is R=t ¼ 500. The geometry andboundary conditions of the plate are shown in Fig. 16. An unstruc-tured mesh composed of 2232 elements is adopted, as depicted inFig. 16(b). The local buckling in tensile loading may occur at crack
Fig. 11. Effect of crack angle and boundary conditions on the buckling stresses.
faces due to the generated local compressive stresses in theseregions. It is illustrated that fiber orientation can have a significanteffect on the buckling loads and mode shapes. Also, different anglesof crack are taken into account and the sensitivity of the results arestudied.
Fig. 17 illustrates the importance of fibers direction on thebuckling load. The crack is considered horizontal and the directionof fibers varies from horizontal to vertical. Clearly, the bucklingloads are substantially sensitive to the orientation of the fibers;for instance for the case of a=2R ¼ 0:6 , the critical buckling loadfor b ¼ 0� is 3.8 times greater than the buckling load for b ¼ 90�.The most vulnerable case occurs when the fibers are perpendicularto the crack path (b ¼ 90�Þ.
Also, a comparison is made for different crack angles to investi-gate the effect of crack orientation on the buckling load. For thispurpose, the crack length is assumed constant a=2R ¼ 0:7. The pre-dicted buckling loads are shown in Fig. 18, which shows that thecrack angle can significantly change the buckling behavior. Adecrease of 52 % occurs in the buckling load for the case ofb ¼ 0�, as the crack angle is increased from h ¼ 30� to h ¼ 45�.
Finally, the buckling mode shapes for the case of a horizontalcrack with a=2R ¼ 0:7 and b ¼ 30� are depicted in Fig. 19.Accordingly, the plate buckles locally only around the crack faceswhere the compressive stresses are generated even in global con-centrated tensile point loadings.
3.5. Composite square plate with two parallel cracks
Due to the fact that XFEM formulation can handle problems ofmultiple cracks, the last example is dedicated to buckling analysisof a composite square plate with two parallel cracks under tensileloading, as shown in Fig. 20. The effects of crack length, distancebetween two cracks and different isotropic and orthotropic tipenrichment functions on the critical buckling stress are investi-gated. The dimensions of the plate are W ¼ 240 mm and t¼ 1 mm and a 35� 35 structured mesh is considered. The bound-ary conditions of the plate is similar to Type-A in Section 3.2.2,direction of the fibers are assumed parallel to the cracks and thematerial properties are similar to other composite examples.
The critical buckling stresses for different crack lengths and dis-tances between the cracks are presented in Table 6. It is observedthat increasing the crack length substantially affects the bucklingbehavior of plate. For example, in all cases, the buckling stressesfor a=W ¼ 0:8 are approximately 6 times lower than the case ofa=W ¼ 0:5. Also, with increasing the distance of cracks, at first,
Fig. 12. Edge cracked plate subjected to shear loading.
Fig. 13. Critical shear force with respect to the normalized crack length.
Fig. 14. Buckling shear stresses of the edge cracked panel for different crack lengthsand fiber angles.
Fig. 15. The first three buckling mode shapes for the edge cracked plate subjectedto shear loading for two different fiber orientations, (a) b ¼ 0� and (b) b ¼ 90� .
Fig. 16. Cracked composite circular plate (a) and the FE mesh (b).
Fig. 17. Buckling loads versus fiber angles for different horizontal crack lengths.
Fig. 18. Effect of crack angle and fiber direction on the buckling load.
A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343 341
the buckling stresses are increased up to d=W ¼ 0:1667, and thendecreased when the cracks approaching to the edges of the plate.
In order to evaluate the effect of different crack tip enrichmentfunctions on plate buckling response two sets of in-plane isotropicand orthotropic tip enrichment functions are considered and theresults are presented in Table 7. It can be noted that with decreas-ing the distance of the cracks the difference between bucklingstresses predicted by adopted isotropic and orthotropic tip enrich-ment functions are increased. The reason can be attributed to thefact that when two crack tips approach, they intensify the stressconcentration in the neighborhood of the crack tips. Such a com-plex displacement field is better captured with the orthotropictip enrichment functions, as their analytical bases are closer tothe generated complex field.
The first four mode shapes of buckling for two different dis-tances of cracks are depicted in Fig. 21. Clearly, it can be noted that
Fig. 19. Four buckling mode shapes of circular cracked composite plate.
Fig. 20. Geometry of composite square plate with two parallel cracks.
Table 6Tensile critical buckling stresses for various crack lengths and distance between twocracks.
d=W a=W
0.5 0.6 0.7 0.8
Mode I buckling stress (MPa)
0.0417 47.03 21.40 10.87 7.200.0833 55.22 23.98 11.91 7.970.1667 62.48 27.50 13.65 9.260.3333 53.67 19.61 12.50 8.46
Table 7Tensile buckling stresses for isotropic and orthotropic tip enrichments for variousdistance of cracks.
d=W Mode I buckling stress (MPa)
Orthotropic enrichment Isotropic enrichment Difference (%)
0.0417 10.87 11.67 7.360.0833 11.91 12.67 6.380.1667 13.65 14.46 5.930.3333 12.5 13.09 4.72
Fig. 21. The first four mode shapes of buckling composite plate with two parallelcracks for two different crack distances (a) d/W = 0.33 and (b) d/W = 0.66.
342 A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343
the distance of the cracks can significantly alter the modes of buck-ling, so that when two cracks getting closer, two sides of cracksbuckle simultaneously, despite of the situation when the cracksare near the edges. Also, as mentioned before, when cracksapproaching to the edges of the plate the buckling stressesdecrease. Unfortunately, no reference solution is available for thiscomplicated problem to be used for verification or comparisonpurposes.
4. Conclusion
Numerical buckling analysis has been performed in this studywithin the framework of the extended finite element method forvarious cracked composite plates. The effects of different parame-ters, such as crack length, crack angle and direction of the fiber onthe buckling behavior of several cracked uni-layer compositeplates have extensively been investigated. The following conclu-sions have been made:
� It is clearly demonstrated that the present method is moreaccurate and efficient than the classical finite element method.Even with substantially fewer elements, in some cases twotimes fewer, more accurate results are achieved.� Generally, for all loading conditions, buckling stresses decrease
with increasing the crack length. For example, when the plate issubjected to compressive loading, increasing the coefficient ofcrack length from c ¼ 0:3 to c ¼ 0:8 leads to 58 % reduction inthe buckling stress. Also, the crack direction has a prominent
A. Nasirmanesh, S. Mohammadi / Composite Structures 131 (2015) 333–343 343
effect on the buckling behavior of the plate. For instance, in thetensile loading condition, when the crack is parallel to the direc-tion of loading, the plate does not buckle.� Fiber directions can significantly change the buckling behavior
of the plate. For example, in the case of rectangular plate sub-jected to tensile loading, changing the fiber direction can alterthe response from the local buckling mode around the crackfaces to a global buckling mode. Also, according to the obtainedresults for the first three examples, it can be observed that themost vulnerable case occurs if the angle of fibers and crack pathis b ¼ 45�.� The present formulation can handle problems of multiple cracks
without any additional difficulties.� The effects of different isotropic and orthotropic tip enrichment
functions on the buckling stresses have been studied. It isobserved that when two crack tips approach, the differencebetween the critical buckling stresses increases. The reasoncan be attributed to the fact that when two crack tip approach,they intensify the stress concentration in the neighborhood ofthe crack tips. Such a complex displacement field is better cap-tured with the orthotropic tip enrichment functions, as theiranalytical bases are chosen to the generated complex field.
Acknowledgments
The authors wish to gratefully acknowledge the technical sup-port of the High Performance Computing Lab, School of CivilEngineering, University College of Engineering, University ofTehran. Furthermore, the financial support of Iran NationalScience Foundation (INSF) is gratefully acknowledged.
References
[1] Thai H-T, Kim S-E. Levy-type solution for buckling analysis of orthotropicplates based on two variable refined plate theory. Compos Struct2011;93:1738–46.
[2] Lopatin A, Morozov E. Buckling of the SSFF rectangular orthotropic plate underin-plane pure bending. Compos Struct 2009;90:287–94.
[3] Bao G, Jiang W, Roberts J. Analytic and finite element solutions for bending andbuckling of orthotropic rectangular plates. Int J Solids Struct1997;34:1797–822.
[4] Lopatin A, Korbut Y. Buckling of clamped orthotropic plate in shear. ComposStruct 2006;76:94–8.
[5] Naderi A, Saidi A. An accurate approach for finding the critical buckling stressof thick orthotropic plates. Compos Struct 2013;96:411–8.
[6] Qiao P, Huo X. Explicit local buckling analysis of rotationally-restrainedorthotropic plates under uniform shear. Compos Struct 2011;93:2785–94.
[7] Thai CH, Ferreira A, Bordas S, Rabczuk T, Nguyen-Xuan H. Isogeometricanalysis of laminated composite and sandwich plates using a new inversetrigonometric shear deformation theory. Eur J Mech A/Solids 2014;43:89–108.
[8] Thai CH, Nguyen-Xuan H, Nguyen-Thanh N, Le TH, Nguyen-Thoi T, Rabczuk T.Static, free vibration, and buckling analysis of laminated composite Reissner–Mindlin plates using NURBS-based isogeometric approach. Int J NumerMethods Eng 2012;91:571–603.
[9] Valizadeh N, Natarajan S, Gonzalez-Estrada OA, Rabczuk T, Bui TQ, Bordas SP.NURBS-based finite element analysis of functionally graded plates: staticbending, vibration, buckling and flutter. Compos Struct 2013;99:309–26.
[10] Markström K, StoÅkers B. Buckling of cracked members under tension. Int JSolids Struct 1980;16:217–29.
[11] Shaw D, Huang Y. Buckling behavior of a central cracked thin plate undertension. Eng Fract Mech 1990;35:1019–27.
[12] Riks E, Rankin C, Brogan F. The buckling behavior of a central crack in a plateunder tension. Eng Fract Mech 1992;43:529–48.
[13] Vafai A, Javidruzi M, Estekanchi H. Parametric instability of edge crackedplates. Thin-walled Struct 2002;40:29–44.
[14] Seifi R, Kabiri AR. Lateral Load effects on buckling of cracked plates undertensile loading. Thin-walled Struct 2013;72:37–47.
[15] Seifi R, Khoda-yari N. Experimental and numerical studies on buckling ofcracked thin-plates under full and partial compression edge loading. Thin-walled Struct 2011;49:1504–16.
[16] Alinia M, Hosseinzadeh S, Habashi H. Numerical modelling for bucklinganalysis of cracked shear panels. Thin-walled Struct 2007;45:1058–67.
[17] Guz A, Dyshel MS. Fracture and buckling of thin panels with edge crack intension. Theor Appl Fract Mech 2001;36:57–60.
[18] Khedmati MR, Edalat P, Javidruzi M. Sensitivity analysis of the elastic bucklingof cracked plate elements under axial compression. Thin-walled Struct2009;47:522–36.
[19] Liu F-L. Differential quadrature element method for buckling analysis ofrectangular Mindlin plates having discontinuities. Int J Solids Struct2001;38:2305–21.
[20] Pan Z, Cheng Y, Liu J. A semi-analytical analysis of the elastic buckling ofcracked thin plates under axial compression using actual non-uniform stressdistribution. Thin-walled Struct 2013;73:229–41.
[21] Baiz P, Natarajan S, Bordas S, Kerfriden P, Rabczuk T. Linear buckling analysisof cracked plates by SFEM and XFEM. J Mech Mater Struct 2012;6:1213–38.
[22] Natarajan S, Baiz PM, Bordas S, Rabczuk T, Kerfriden P. Natural frequencies ofcracked functionally graded material plates by the extended finite elementmethod. Compos Struct 2011;93:3082–92.
[23] Nguyen-Thoi T, Rabczuk T, Lam-Phat T, Ho-Huu V, Phung-Van P. Free vibrationanalysis of cracked Mindlin plate using an extended cell-based smootheddiscrete shear gap method (XCS-DSG3). Theor Appl Fract Mech2014;72:150–63.
[24] Yu T, Bui TQ, Liu P, Hirose S. A stabilized discrete shear gap extended finiteelement for the analysis of cracked Reissner–Mindlin plate vibration problemsinvolving distorted meshes. Int J Mech Mater Des 2014:1–23.
[25] Barut A, Madenci E, Britt V, Starnes Jr J. Buckling of a thin, tension-loaded,composite plate with an inclined crack. Eng Fract Mech 1997;58:233–48.
[26] Rad AA, Panahandeh-Shahraki D. Buckling of cracked functionally gradedplates under tension. Thin-walled Struct 2014;84:26–33.
[27] Natarajan S, Chakraborty S, Ganapathi M, Subramanian M. A parametric studyon the buckling of functionally graded material plates with internaldiscontinuities using the partition of unity method. Eur J Mech A/Solids2014;44:136–47.
[28] Asadpoure A, Mohammadi S. Developing new enrichment functions for cracksimulation in orthotropic media by the extended finite element method. Int JNumer Methods Eng 2007;69:2150–72.
[29] Asadpoure A, Mohammadi S, Vafai A. Crack analysis in orthotropic media usingthe extended finite element method. Thin-walled Struct 2006;44:1031–8.
[30] Asadpoure A, Mohammadi S, Vafai A. Modeling crack in orthotropic mediausing a coupled finite element and partition of unity methods. Finite Elem AnalDes 2006;42:1165–75.
[31] Ashari S, Mohammadi S. Delamination analysis of composites by neworthotropic bimaterial extended finite element method. Int J Nume MethodsEng 2011;86:1507–43.
[32] Bayesteh H, Mohammadi S. XFEM fracture analysis of shells: The effect ofcrack tip enrichments. Comput Mater Sci 2011;50:2793–813.
[33] Bayesteh H, Mohammadi S. XFEM fracture analysis of orthotropic functionallygraded materials. Compos Part B: Eng 2013;44:8–25.
[34] Belytschko T, Moës N, Usui S, Parimi C. Arbitrary discontinuities in finiteelements. Int J Numer Methods Eng 2001;50:993–1013.
[35] Dolbow J, Gosz M. On the computation of mixed-mode stress intensity factorsin functionally graded materials. Int J Solids Struct 2002;39:2557–74.
[36] Motamedi D, Mohammadi S. Dynamic crack propagation analysis oforthotropic media by the extended finite element method. Int J Fract2010;161:21–39.
[37] Motamedi D, Mohammadi S. Dynamic analysis of fixed cracks in compositesby the extended finite element method. Eng Fract Mech 2010;77:3373–93.
[38] Motamedi D, Mohammadi S. Fracture analysis of composites by timeindependent moving-crack orthotropic XFEM. Int J Mech Sci 2012;54:20–37.
[39] Nguyen-Thanh N, Valizadeh N, Nguyen M, Nguyen-Xuan H, Zhuang X, Areias P,et al. An extended isogeometric thin shell analysis based on Kirchhoff–Lovetheory. Comput Methods Appl Mech Eng 2015;284:265–91.
[40] Rabczuk T, Areias P. A meshfree thin shell for arbitrary evolving cracks basedon an extrinsic basis. 2006.
[41] Rabczuk T, Areias P, Belytschko T. A meshfree thin shell method for non-lineardynamic fracture. Int J Numer Methods Eng 2007;72:524–48.
[42] Mohammadi S. Extended finite element method: for fracture analysis ofstructures. John Wiley & Sons; 2008.
[43] Mohammadi S. XFEM fracture analysis of composites. John Wiley & Sons;2012.
[44] Lekhnitskii S. Theory of elasticity of an anisotropic elastic body. SanFrancisco: Holden-Day; 1963.
[45] Cook RD. Concepts and applications of finite element analysis. John Wiley &Sons; 2007.
[46] Bordas S, Natarajan S, Kerfriden P, Augarde CE, Mahapatra DR, Rabczuk T, et al.On the performance of strain smoothing for quadratic and enriched finiteelement approximations (XFEM/GFEM/PUFEM). Int J Numer Methods Eng2011;86:637–66.
[47] Mousavi S, Sukumar N. Numerical integration of polynomials anddiscontinuous functions on irregular convex polygons and polyhedrons.Comput Mech 2011;47:535–54.
[48] Natarajan S, Bordas S, Roy Mahapatra D. Numerical integration over arbitrarypolygonal domains based on Schwarz–Christoffel conformal mapping. Int JNumer Methods Eng 2009;80:103–34.
[49] Natarajan S, Mahapatra DR, Bordas S. Integrating strong and weakdiscontinuities without integration subcells and example applications in anXFEM/GFEM framework. Int J Numer Methods Eng 2010;83:269–94.
[50] Ventura G, Gracie R, Belytschko T. Fast integration and weight functionblending in the extended finite element method. Int J Numer Methods Eng2009;77:1–29.